notebook PCs. Current research and development at .... battery cell attachment, contact your Rigaku sales or service representative). Figure 5 shows an ...
Battery cell attachment —In situ X-ray diffractometry for observations of structural change in electrode materials during charging and discharging— 1.
Introduction Lithium ion secondary batteries (LIBs) are widely used in compact mobile devices such as cell phones and notebook PCs. Current research and development at universities, research institutions, and companies seek to create LIBs for use in large machines, including electric vehicles. Meanwhile, competition in the development of LIBs has intensiﬁed in Asian and Western countries. Commercializing LIBs requires improvements in capacity, stability, and longevity, which in turn entail various assessments and evaluations. Figure 1 shows aspects of LIBs that equipment manufactured and sold by Rigaku can be used to assess. Among the evaluation methods currently available, X-ray diffractometry offers a wide range of analytical capabilities that allows extensive examination of structural changes in electrode materials, such as qualitative analysis, crystallite size analysis, and Rietveld analysis. At the 50th Battery Symposium in Japan, held in 2009, half a dozen reports were presented on in situ measurements of LIBs by various analytical methods. In contrast, at the 51st Battery Symposium in Japan, held in November 2010 in Nagoya, the number of reports on in situ measurements of LIBs numbered 18, a threefold increase. Announced at this most recent symposium were the results of experiments done at SPring-8. The
Fig. 1. 32
results of measurements of structural changes obtained with X-ray diffractometers while batteries are charged and discharged point to structural changes in electrode materials, even during the initial charge/discharge cycle; lithium desorption and insertion at certain points during the charge/discharge cycle; and other details, such as changes in bond distances between metal and oxygen atoms. Additionally, much work related to in situ evaluations is being done today in laboratory environments. The results of laboratory analyses using the battery cell attachment discussed in this paper have been reported at the 78th Meeting of the Electrochemical Society of Japan(1) in March 2011.
Measuring LIBs in the charge/discharge state Since LIBs undergo repeated charge and discharge cycles, evaluations using an X-ray diffractometer must be done while LIBs are being charged or discharged. Ex situ measurements or in situ measurements are used to evaluate LIBs in the charge/discharge state. For ordinary ex situ measurements, coin cells are repeatedly charged and discharged under speciﬁc conditions. The cells are then taken apart and examined by X-ray diffraction analysis or other methods. This approach poses the following issues:
Lithium ion battery evaluation.
The Rigaku Journal, 27(2), 2011
External view of battery cell attachment.
(1) Many coin cells must be prepared for these charge/discharge tests. Once a coin cell is taken apart, it cannot be charged or discharged. Therefore, many test cells must be prepared, resulting in the need to account for variations from cell to cell and variations among tests done by different testing personnel. (2) Material stability problem during disassembly. When the components of a LIB are exposed to oxygen or moisture, they may degrade or undergo reactions. This means certain awkward procedures must be done in a glove box (bag). (3) There is no way to determine if the disassembly affects the charge/discharge state. Disassembly may result in natural discharge.
Sample setup procedure.
By comparison, in situ measurements make it possible to analyze LIBs in their original condition without taking them apart, eliminating concerns related to the issues above.
Overview and features of the Rigaku-manufactured battery cell attachment Figure 2 is an external view of the Rigaku battery cell attachment. Figure 3 shows the sample setup procedure. Figure 4 shows the battery cell attachment mounted on an X-ray diffractometer.
3.1. Main speciﬁcation • Sample dimensions: Positive electrode diameter (standard) 15 to 16 mm (formed on aluminum foil or mesh) Negative electrode diameter (standard) 18 to 19 mm Separator diameter 20.0 to 20.5 mm • 2q angle range: From 10° • Main body material: Stainless steel • Insulating material: Teﬂon • Window material: Beryllium • Number of poles, electrode materials: 2 poles (positive electrode: beryllium, negative electrode: stainless steel) • Sealing material: O-ring • Pressing and retaining the sample: After setting the The Rigaku Journal, 27(2), 2011
Fig. 4. Example: Mounting the battery cell attachment on an X-ray diffractometer.
spacer and wave washer into position, use a quick clamp to hold the sample in place. • Rated voltage and current: 32 VDC, 3 A max. • Terminal: Equipped with two-pole terminal for charge/ discharge A sample is set up in the battery cell attachment inside a glove box as shown in Fig. 3. With the beryllium window facing down, the positive electrode material, separator, and negative electrode are set in place, in that sequence. Electrolyte is added, if needed. 33
Battery cell attachment
Example of measurement of lithium cobalt oxide sample.
X-ray diffraction proﬁles of LiFePO4 during charge process.
The spacer and wave washer are placed on top, and the metal retainer and other parts are mounted. A quick clamp is used to hold the assembly. Figure 2 shows a sample held by a quick clamp. The battery cell attachment with a sample mounted as described above is set on the attachment mounting base of the X-ray diffractometer (Fig. 4).
Main applications and features of battery cell attachment The battery cell attachment discussed here allows Xray diffraction measurement of the battery mounted in the battery cell attachment. It does not require removal of the sample. This makes it suitable for measuring
structural changes in electrode materials while varying the charge/discharge conditions in ﬁne steps during the initial charge/discharge cycle, or during the ﬁrst several cycles, rather than for observations of structural change in the electrode materials of a coin battery over the course of several dozen or more charge/discharge cycles. Rigaku developed the battery cell attachment after consulting LIB researchers with extensive experience in the area. For example, the battery cell attachment is conﬁgured so that a battery can be mounted in the attachment easily and securely in a glove box, without screws. It allows measurement from 2q ⫽10°, and is capable of detecting positive electrode degradation signals in a low angle range. The Rigaku Journal, 27(2), 2011
The battery cell attachment can be mounted on several Rigaku X-ray diffractometers, including SmartLab, TTRAX III, Ultima IV, and D/MAX. (To determine if your equipment is compatible with the battery cell attachment, contact your Rigaku sales or service representative). Figure 5 shows an example of results from measuring a lithium cobalt oxide sample at a scan speed of 50°/min using a high-speed one-dimensional detector (measuring equipment: TTRAX III, X-ray source: 50 kV, 300 mA).
Example of in situ measurement using the battery cell attachment The advantages offered by olivine-type LiFePO4 include low environmental impact and excellent thermal stability, prompting study for use as a positive electrode material for batteries for automobiles and large machinery. We evaluated the crystal structure of LiFePO4 during a charge process using the battery cell attachment (samples courtesy of Professor Tatsuya Nakamura, Graduate School of Engineering, University of Hyogo). We set LiFePO4 in the battery cell attachment and performed X-ray diffraction measurements at states of charge (SOC) of 0, 40, 60, 80, and 100%. Figure 6 shows the X-ray diffraction proﬁle and qualitative analysis results at each SOC. Only single-phase LiFePO4
The Rigaku Journal, 27(2), 2011
was observed at the 0% SOC, but as the SOC increased, diffracted X-rays deriving from FePO4 began to appear. At the 100% SOC, diffracted X-rays showed a nearcomplete FePO4 phase transition, indicating a two-phase reaction between LiFePO4 and FePO4 in the LiFePO4 in the charged state.
Summary At the 51st Battery Symposium in Japan held last fall, researchers involved in state of the art work stressed that clarifying the positive electrode degradation mechanism would require detailed examination of structural changes in the positive electrode from various perspectives during the initial charge and discharge cycle. Continuing progress in the research, development, and industrialization of lithium ion secondary batteries offering high performance, longevity, cost-effectiveness, and safety are strongly needed to mitigate everincreasing serious environmental problems. It is our hope that the battery cell attachment introduced in this paper will contribute to these efforts. Reference (1)
Tatsuya Nakamura, Shin-ichi Masuda, Yuya Shima, Akari Takahara and Hisashi Yashiro: Proceedings of the Academic Lecture Session of the 78th Meeting of The Electrochemical Society of Japan, (2011), 2L04.